Published on Web 03/09/2004
Synthesis and Electronic Properties of Donor-Acceptor π-Conjugated Siloles A. J. Boydston, Youshi Yin, and Brian L. Pagenkopf* Department of Chemistry and Biochemistry, The UniVersity of Texas at Austin, Austin, Texas 78712 Received January 14, 2004; E-mail: [email protected]
Siloles are being increasingly recognized as promising and desirable π-conjugated materials for potential device applications, and important contributions have been made in the areas of electroand photoluminescence1 and nitroaromatic sensors.2 They are also strong candidates for NLO applications based on the theoretical works of Matsuzaki3 and Bakhshi4 and the successes with related arylene materials.5 The ability to control the electronic nature of the silole chromophore by varying the functional groups at the silole termini will be critical to fine-tuning and optimizing their properties. Access to silole systems bearing electron donating and accepting groups peripherally at the C(2) and C(5) positions has been impeded by the challenges of synthesizing desymmetrized siloles. The synthesis of functionalized 2,5-silole extended chromophores is notoriously complicated by the incompatibility of the silole ring with traditional alkyne protecting groups. For example, the nucleophilic nature of the reaction conditions present during removal of conventional orthogonal alkyne protecting groups (e.g., Me3Si vs iPr3Si vs Me2COH) successfully employed in the synthesis of other acetylenic systems6 results in rapid desilylation of the silole moiety.1f,7 In pioneering investigations, Tamao prepared asymmetric siloles suitable for further functionalization by monolithiation of a symmetrical 2,5-dibromosilole, followed by electrophilic trapping.8 We sought a more direct route to obtain asymmetric siloles through site-specific cross-coupling methodology. Utilizing ZnCl2 as an oxidizing agent for residual LiNaph, an approach that has proven advantageous in Negishi silole cross-couplings involving aryl halides,1f provided a satisfying 84% isolated yield of 2,5-dibromosilole 3 (Scheme 1).9 However, our efforts to desymmetrize the dibromosilole 3 by selective single cross-coupling reactions failed, and formation of the undesired biscoupled product along with unreacted starting material was the usual result. Attempts to desymmetrize the dizinc intermediate 2 by low temperature monobromination were stymied by formation of only the dibromosilole. We suspected that chlorination might be superior to bromination given the greater deactivating effect expected from a monochlorosilole on the nucleophilicity of the second vinyl zinc. However, chlorination of 2 using N-chlorosuccinimide gave fickle results with poor ratios of mono- to dichlorosilole (1.1:1, 84% combined yield). In contrast, successful monochlorination (16.2:1 ratio) was achieved using N-chlorophthalimide (NCP), and the intermediate 2-chloro-5metallosilole 4 could be further functionalized by iodination with I2 to afford the new chloroiodosilole 5 in 81% yield (Scheme 2). The high light sensitivity of 5 complicated its isolation and storage, but through extensive optimization we have found in situ crosscoupling reactions to be extraordinarily useful for asymmetric silole synthesis. The best results were obtained by engaging the electronpoor acceptor alkyne in the first cross-coupling event at 40 °C, and when complete (ca. 14 h), the donor moieties were allowed to react at 70 °C. In this way, donor-acceptor (DA) systems 7-15 have each been prepared by an operationally simple process requiring only a single purification step (Scheme 2 and Table 1).10 Specifically, the entire sequence consisting of cycloreduction, 3724
J. AM. CHEM. SOC. 2004, 126, 3724-3725
Table 1. Summary of Data for Donor-Acceptor Siloles silole
absorption λmax (log )
emission λmax (ΦF × 10-2)a
6 7 8 9 10 11 12 13 14 15
H OCH3 OCH3 NH2 OCH3 NH2 NMe2 NH2 NMe2 NMe2
H H CN H NO2 CN H NO2 CN NO2
429 (4.74) 435 (4.33) 443 (4.33) 445 (4.51) 456 (4.44) 457 (4.44) 465 (4.25) 471 (4.11) 476 (4.53) 496 (4.37)
520 (8.97) 528 (4.06) 559 (0.70) 558 (2.57) 649 (0.44) 594 (1.80) 598 (2.12) 613 (0.11) 611 (2.94) nde
82c 65 54 62 55 58 55 56 58 54
-d Pbnc P21/c -d P1h Pna21 -d Pna21 P21/c P21/c
a Determined with reference to fluorescein. b Isolated yields based on diethynylsilane 1. c Isolated yield based on dibromosilole 3. d Suitable crystals not yet obtained. e Photoluminescence not detected.
transmetalation, chlorination, iodination, and two sequential crosscouplings produced asymmetric siloles 7-15 in 54-65% isolated overall yield based on diyne 1. These materials are the first silole-containing extended chromophores bearing electronically dissimilar functional groups at C(2) and C(5) prepared by direct cross-coupling methodology. In this regard, a disincentive to large-scale silole synthesis by crosscoupling methodology was its previous reliance on stoichiometric tin reagents11 for Stille-type12 chemistry. Alkyne cross-couplings with 2,5-dihalo siloles under related Sonogashira conditions13 proved fickle in our hands, as observed by others.7,14 To the best of our knowledge, this communication constitutes the first successful alkyne cross-couplings under Negishi conditions.15 The electronic absorption spectra of DA siloles 7-15, along with the parent compound 6,10 are shown in Figure 1. All of the compounds absorb in the visible region, and absorption maxima strongly depend on the nature of the push-pull substituents of the chromophore. Sequentially increasing the degree of electron delocalization from the parent silole 6 (A ) D ) H) to the most polar silole (15) results in a stepwise bathochromic shift in the electronic absorption spectra from 429 to 496 nm. These results demonstrate experimentally that silole chromophores can be electronically fine10.1021/ja049758z CCC: $27.50 © 2004 American Chemical Society
Figure 1. Electronic absorption spectra of donor-acceptor siloles in CH2Cl2.
trosymmetric space groups. This is particularly evident in comparing the amino siloles (11 and 13) with the dimethylamino counterparts (14 and 15) in which a hydrogen bond donor is absent. Further exploitation of hydrogen bonding directed crystal packing with other DA systems is currently underway in our laboratory. In summary, we have developed a new and efficient method for the synthesis of novel donor-acceptor silole chromophores by direct cross-coupling reactions. The ability to manipulate the electronic and physical properties of siloles through judicious combinations of peripheral functional groups was also demonstrated. The entire synthetic sequence from silane 1 to DA systems is achieved efficiently in two steps with only a single purification process. Silole alkene cross-couplings and utilization of 5 to prepare secondgeneration siloles will be described elsewhere. Acknowledgment. We thank the Robert A. Welch Foundation and donors of the American Chemical Society Petroleum Research Fund for partial financial support of this research. We thank Dr. Vincent Lynch for determination of crystal structures and Professors Allen Bard, David Vanden Bout, and Grant Willson for helpful discussions. Y.Y. thanks Pfizer for an undergraduate research fellowship. Supporting Information Available: Detailed experimental procedures (PDF) and characterization of all new compounds (CIF). This material is available free of charge via the Internet at http://pubs.acs.org.
Figure 2. Photoluminescence spectra of donor-acceptor siloles in CH2Cl2.
Figure 3. X-ray structure of silole 13. Hydrogen bonds are shown in red.
tuned by the manipulation of peripheral DA functional groups. This advance brings siloles into the family of electronically tunable DA chromophores. The consequences of varying the nature of the DA groups are also manifested in the photoluminescence spectra (Figure 2). Interestingly, silole 10 (D ) OCH3, A ) NO2) exhibits only the fifth longest wavelength absorption in this series, but displays the longest wavelength emission at 649 nm.16 This is the longest wavelength emission for a compound possessing only a single silole in the chromophore.1f The moderate silole quantum efficiencies (Table 1) are consistent with previous observations.1f Siloles 7, 8, 10, 11, and 13-15 gave crystals suitable for X-ray analysis (Table 1). Curiously, only 11 and 13 packed in a noncentrosymmetric space group (Pna21, Figure 3).17 Within these crystals, two sheets of siloles intersect at 45°, and the orientation of the dimethylsilylene moiety is unidirectional throughout. The DA groups within a sheet reinforce the induced dipole by aligning in a head-to-tail fashion, and the intersecting sheet is oriented in an electrostatically complementary direction. In contrast, the remaining compounds packed in centrosymmetric space groups in which the dimethylsilylene moiety and the DA groups pack in a head-to-head orientation that minimizes dipoles. We speculate that hydrogen bonding facilitates noncentrosymmetric packing in 11 and 13. The average hydrogen bond distances and bond angles in 11 and 13 are 2.122 Å, 170° and 2.107 Å, 148°, respectively. In contrast, dipole-directed packing will favor cen-
References (1) For selected examples, see: (a) Chen, J.; Law, C. C. W.; Lam, J. W. Y.; Dong, Y.; Lo, S. M. F.; Williams, I. D.; Zhu, D.; Tang, B. Z. Chem. Mater. 2003, 15, 1535-1546. (b) Kim, B.-H.; Woo, H.-G. Organometallics 2002, 21, 2796-2798. (c) Uchida, M.; Izumizawa, T.; Nakano, T.; Yamaguchi, S.; Tamao, K.; Furukawa, K. Chem. Mater. 2001, 13, 2680-2683. (d) Yamaguchi, S.; Endo, T.; Uchida, M.; Izumizawa, T.; Furukawa, K.; Tamao, K. Chem. Lett. 2001, 30, 98-99. (e) Tamao, K.; Uchida, M.; Izumizawa, T.; Furukawa, K.; Yamaguchi, S. J. Am. Chem. Soc. 1996, 118, 11974-11975. (f) Yamaguchi, S.; Endo, T.; Uchida, M.; Izumizawa, T.; Furukawa, K.; Tamao, K. Chem.-Eur. J. 2000, 6, 16831692. (2) (a) Sohn, H.; Sailor, M. J.; Magde, D.; Trogler, W. C. J. Am. Chem. Soc. 2003, 125, 3821-3830. (b) Sohn, H.; Calhoun, R. M.; Sailor, M. J.; Trogler, W. C. Angew. Chem., Int. Ed. 2001, 40, 2104-2105. (3) Matsuzaki, Y.; Nakano, M.; Yamaguchi, K.; Tanaka, K.; Yamabe, T. Chem. Phys. Lett. 1996, 263, 119-125. (4) Gandhi, G.; Bakhshi, A. K. Solid State Commun. 2003, 128, 467-472. (5) Nonlinear Optical Effects and Materials; Gu¨nter, P., Ed.; Springer: Heidelberg, Germany, 2000. (6) (a) Nielsen, M. B.; Utesch, N. F.; Moonen, N. N. P.; Boudon, C.; Gisselbrecht, J.-P.; Concilio, S.; Piotto, S. P.; Seiler, P.; Gunter, P.; Gross, M.; Diederich, F. Chem.-Eur. J. 2002, 8, 3601-3613. (b) Blanchette, H. S.; Brand, S. C.; Naruse, H.; Weakley, T. J. R.; Haley, M. M. Tetrahedron 2000, 56, 9581-9588. (c) Cuilei, S. C.; Tykwinski, R. R. Org. Lett. 2000, 2, 3607-3610. (d) Wan, W. B.; Brand, S. C.; Pak, J. J.; Haley, M. M. Chem.-Eur. J. 2000, 6, 2044-2052. (e) De Nicola, A.; Ringenbach, C.; Ziessel, R. Tetrahedron Lett. 2003, 44, 183-187. (f) Tour, J. M. Chem. ReV. 1996, 96, 537-553. (g) Moore, J. S. Acc. Chem. Res. 1997, 30, 402-413. (7) Yamaguchi, S.; Iimura, K.; Tamao, K. Chem. Lett. 1998, 27, 89-90. (8) Tamao, K.; Yamaguchi, S.; Shiro, M. J. Am. Chem. Soc. 1994, 116, 11715-11722. (9) Halogenation from the dizinc was more efficient and consistent than that from the dilithio species; see ref 8. (10) Compounds exactly analogous to 6 have been prepared from 2,5dibromosiloles; see refs 7 and 8. (11) (a) Chen, W.; Ijadi-Maghsoodi, S.; Barton, T. Polym. Prepr. (Am. Chem. Soc., DiV. Polym. Chem.) 1997, 38, 189-190. (b) For a mini review, see: Yamaguchi, S.; Tamao, K. J. Organomet. Chem. 2002, 653, 223-228. (12) Stille, J. K.; Simpson, J. H. J. Am. Chem. Soc. 1987, 109, 2138-2152. (13) Sonogashira, K.; Tohda, Y.; Hagihara, N. Tetrahedron Lett. 1975, 16, 4467-4470. (14) Ohshita, J.; Mimura, N.; Arase, H.; Nodono, M.; Kunai, A.; Komaguchi, K.; Shiotani, M.; Ishikawa, M. Macromolecules 1998, 31, 7985-7987. (15) For a modified procedure that does not require anhydrous conditions, see: Anastasia, L.; Negishi, E. Org. Lett. 2001, 3, 3111-3113. (16) The emission λmax and quantum yield remained consistent over a broad concentration range (0.1-45 µM). (17) It is encouraging that both aminosiloles display noncentrosymmetric packing, which is a requirement for second-harmonic generation in the solid state; see ref 5.
J. AM. CHEM. SOC.
VOL. 126, NO. 12, 2004 3725